The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R


 Bethany Phelps
 3 years ago
 Views:
Transcription
1 3.5 Show that the atomic packing factor for BCC is The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated with each unit cell for BCC V S 4πR 8πR = 2(sphere volume) = 2 = Also, the unit cell has cubic symmetry, that is V C = a 3. But a depends on R according to Equation 3.3, and Thus, V C = 4R 3 3 = 64 R VS 8 π R /3 APF = = = V 64 R / 3 3 C
2 3.61 The metal iridium has an FCC crystal structure. If the angle of diffraction for the (220) set of planes occurs at (firstorder reflection) when monochromatic xradiation having a wavelength of nm is used, compute (a) the interplanar spacing for this set of planes, and (b) the atomic radius for an iridium atom. (a) From the data given in the problem, and realizing that = 2θ, the interplanar spacing for the (220) set of planes for iridium may be computed using Equation 3.13 as d 220 nλ (1)(0.154 nm) = = = 2sinθ (2) sin nm (b) In order to compute the atomic radius we must first determine the lattice parameter, a, using Equation 3.14, and then R from Equation 3.1 since Ir has an FCC crystal structure. Therefore, ( ) a = d + + = = (2) (2) (0) ( nm) nm And, from Equation 3.1 a nm R = = = nm
3 4.2 Calculate the number of vacancies per cubic meter in iron at 855 C. The energy for vacancy formation is 1.08 ev/atom. Furthermore, the density and atomic weight for Fe are 7.65 g/cm 3 and g/mol, respectively. Determination of the number of vacancies per cubic meter in iron at 855 C (1128 K) requires the utilization of Equations 4.1 and 4.2 as follows: N Q N ρ Qv exp exp kt A kt v A Fe v = N = Fe And incorporation of values of the parameters provided in the problem statement into the above equation leads to Nv ( )( ) atoms / mol 7.65 g / cm 1.08 ev / atom = exp g / mol ( ev / atom K )(1128 K) = cm 3 = m 3
4 5.7 A sheet of steel 1.8 mm thick has nitrogen atmospheres on both sides at 1200 C and is permitted to achieve a steadystate diffusion condition. The diffusion coefficient for nitrogen in steel at this temperature is m 2 /s, and the diffusion flux is found to be kg/m 2 s. Also, it is known that the concentration of nitrogen in the steel at the highpressure surface is 4 kg/m 3. How far into the sheet from this highpressure side will the concentration be 2.0 kg/m 3? Assume a linear concentration profile. This problem is solved by using Equation 5.3 in the form J = D C A C B x A x B If we take C A to be the point at which the concentration of nitrogen is 4 kg/m 3, then it becomes necessary to solve for x B, as x B = x A + D C A C B J Assume x A is zero at the surface, in which case x 4 kg / m 2 kg / m kg / m s B = 0 + ( 6 10 m /s) = m = 1 mm
5 5.22 The diffusion coefficients for silver in copper are given at two temperatures: T ( C) D (m 2 /s) (a) Determine the values of D 0 and Q d. (b) What is the magnitude of D at 875 C? (a) Using Equation 5.9a, we set up two simultaneous equations with Q d and D 0 as unknowns as follows: ln D 1 = lnd 0 Q d 1 R T 1 ln D 2 = lnd 0 Q d R 1 T 2 Solving for Q d in terms of temperatures T 1 and T 2 (923 K [650 C] and 1173 K [900 C]) and D 1 and D 2 ( and m 2 /s), we get Q d = R ln D 1 ln D 2 1 T 1 1 T 2 = ( ) ( ) (8.31 J/mol K) ln ln K 1173 K = 196,700 J/mol Now, solving for D 0 from Equation 5.8 (and using the 650 C value of D) D 0 = D 1 exp Q d RT , 700 J/mol = ( m /s) exp (8.31 J/mol K)(923 K) = m 2 /s
6 (b) Using these values of D 0 and Q d, D at 1148 K (875 C) is just , 700 J/mol D = ( m /s) exp (8.31 J/mol K)(1148 K) = m 2 /s Note: this problem may also be solved using the Diffusion module in the VMSE software. Open the Diffusion module, click on the D 0 and Q d from Experimental Data submodule, and then do the following: 1. In the lefthand window that appears, enter the two temperatures from the table in the book (converted from degrees Celsius to Kelvins) (viz. 923 (650ºC) and 1173 (900ºC), in the first two boxes under the column labeled T (K). Next, enter the corresponding diffusion coefficient values (viz. 5.5e16 and 1.3e13 ). 3. Next, at the bottom of this window, click the Plot data button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence for this diffusion system. At the top of this window are give values for D 0 and Q d ; for this specific problem these values are m 2 /s and 196 kj/mol, respectively 5. To solve the (b) part of the problem we utilize the diamondshaped cursor that is located at the top of the line on this plot. Clickanddrag this cursor down the line to the point at which the entry under the Temperature (T): label reads 1148 (i.e., 875ºC). The value of the diffusion coefficient at this temperature is given under the label Diff Coeff (D):. For our problem, this value is m 2 /s.
7 StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 12 mm 12.9 mm is pulled in tension with 35,600 N force, producing only elastic deformation. Calculate the resulting strain. This problem calls for us to calculate the elastic strain that results for an aluminum specimen stressed in tension. The crosssectional area is just (12 mm) (12.9 mm) = 155 mm 2 (= m 2 ); also, the elastic modulus for Al is given in Table 6.1 as 69 GPa (or N/m 2 ). Combining Equations 6.1 and 6.5 and solving for the strain yields σ F 35,600 N = = = = E A E ( m )( N/m ) 3
8 7.23 (a) From the plot of yield strength versus (grain diameter) 1/2 for a 70 Cu 30 Zn cartridge brass, Figure 7.15, determine values for the constants σ 0 and k y in Equation 7.7. (b) Now predict the yield strength of this alloy when the average grain diameter is mm. (a) Perhaps the easiest way to solve for σ 0 and k y in Equation 7.7 is to pick two values each of σ y and d 1/2 from Figure 7.15, and then solve two simultaneous equations, which may be created. For example d 1/2 (mm) 1/2 σ y (MPa) The two equations are thus σ 75 = k y σ 175 = k y of these equations yield the values of k y 1/2 = 12.5 MPa (mm) σ 0 = 25 MPa (b) When d = mm, d 1/2 = mm 1/2, and, using Equation 7.7, σ y = σ + 0 kd y 1/2 ( ) 1/2 1/2 = (25 MPa) MPa (mm) mm = 305 MPa
9 8.8 A large plate is fabricated from a steel alloy that has a plane strain fracture toughness of 55 MPa m. If, during service use, the plate is exposed to a tensile stress of 200 MPa, determine the minimum length of a surface crack that will lead to fracture. Assume a value of 1.0 for Y. For this problem, we are given values of K Ic ( 55 MPa m), σ (200 MPa), and Y (1.0) for a large plate and are asked to determine the minimum length of a surface crack that will lead to fracture. All we need do is to solve for a c using Equation 8.7; therefore a c 2 1 KIc 1 55 MPa m = m 24 mm π = = = Y σ π (1.0)(200 MPa) 2
10 Cyclic Stresses (Fatigue) The SN Curve 8.14 A fatigue test was conducted in which the mean stress was 50 MPa and the stress amplitude was 225 MPa. (a) Compute the maximum and minimum stress levels. (b) Compute the stress ratio. (c) Compute the magnitude of the stress range. (a) Given the values of σ m (50 MPa) and σ a (225 MPa) we are asked to compute σ max and σ min. From Equation 8.14 Or, σ m σ + σ 2 max min = = 50 MPa σ max + σ min = 100 MPa Furthermore, utilization of Equation 8.16 yields σ a = σ max σ min 2 = 225 MPa Or, σ max σ min = 450 MPa Simultaneously solving these two expressions leads to σ = 275 MPa max σ = 175 MPa min (b) Using Equation 8.17 the stress ratio R is determined as follows: R σ σ min = = = max 175 MPa 275 MPa 0.64
11 (c) The magnitude of the stress range σ r is determined using Equation 8.15 as σ r = σmax σmin = 275 MPa ( 175 MPa) = 450 MPa
12 9.32 For a copper silver alloy of composition 30 wt% Ag 70 wt% Cu and at 775 C (1048 K) do the following: (a) Determine the mass fractions of α and β phases. (b) Determine the mass fractions of primary α and eutectic microconstituents. (c) Determine the mass fraction of eutectic α. (a) This portion of the problem asks that we determine the mass fractions of α and β phases for an 30 wt% Ag 70 wt% Cu alloy (at 775 C (1048 K)). In order to do this it is necessary to employ the lever rule using a tie line that extends entirely across the α + β phase field. From Figure 9.7 and at 775 C (1048 K), C α = 8.0 wt% Ag, C β = 91.2 wt% Ag, and C eutectic = 71.9 wt% Sn. Therefore, the two lever rule expressions are as follows: Cβ C Wα = = = C C β α C0 Cα Wβ = = = C C β α (b) Now it is necessary to determine the mass fractions of primary α and eutectic microconstituents for this same alloy. This requires us to utilize the lever rule and a tie line that extends from the maximum solubility of Ag in the α phase at 775 C (1048 K) (i.e., 8.0 wt% Ag) to the eutectic composition (71.9 wt% Ag). Thus W α Ceutectic C = = = C C eutectic α C C = = = α We C eutectic C α (c) And, finally, we are asked to compute the mass fraction of eutectic α, W eα. This quantity is simply the difference between the mass fractions of total α and primary α as W = W W = = 0.08 eα α α
13 10.8 It is known that the kinetics of recrystallization for some alloy obey the Avrami equation and that the value of n in the exponential is 2.5. If, at some temperature, the fraction recrystallized is 0.50 after 200 min, determine the rate of recrystallization at this temperature. This problem gives us the value of y (0.40) at some time t (200 min), and also the value of n (2.5) for the recrystallization of an alloy at some temperature, and then asks that we determine the rate of recrystallization at this same temperature. It is first necessary to calculate the value of k. We first rearrange Equation as exp( kt n ) = 1 y and then take natural logarithms of both sides: kt n = ln (1 y) Now solving for k gives k = ln (1 y) t n which, using the values cited above for y, n, and t yields ln (1 0.50) k = = (200 min) 6 At this point we want to compute t 0.5, the value of t for y = 0.5, which means that it is necessary to establish a form of Equation in which t is the dependent variable. From one of the above equations t n = ln (1 y) k And solving this expression for t leads to t = ln (1 y) k 1/ n
14 For t 0.5, this equation takes the form t 0.5 ln (1 0.5) = k 1/ n and incorporation of the value of k determined above, as well as the value of n cited in the problem statement (2.5), then t 0.5 is equal to t /2.5 ln (1 0.5) = = min Therefore, from Equation 10.18, the rate is just 1 1 rate = = = (min) t min
15 10.18 Using the isothermal transformation diagram for an iron carbon alloy of eutectoid composition (Figure 10.22), specify the nature of the final microstructure (in terms of microconstituents present and approximate percentages of each) of a small specimen that has been subjected to the following time temperature treatments. In each case assume that the specimen begins at 760 C (1033 K) and that it has been held at this temperature long enough to have achieved a complete and homogeneous austenitic structure. (a) Cool rapidly to 700 C (973 K), hold for 10 4 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment. After cooling and holding at 700 C for 10 4 s, approximately 50% of the specimen has transformed to coarse pearlite. Upon cooling to room temperature, the remaining 50% transforms to martensite. Hence, the final microstructure consists of about 50% coarse pearlite and 50% martensite. (b) Reheat the specimen in part (a) to 700 C (973 K) for 20 h. Heating to 700 C for 20 h the specimen in part (a) will transform the coarse pearlite and martensite to spheroidite.
16 (c) Rapidly cool to 600 C (873 K), hold for 4 s, rapidly cool to 448 C (721 K), hold for 10 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment. After cooling to and holding at 600 C for 4 s, approximately 50% of the specimen has transformed to pearlite (medium). During the rapid cooling to 448 C no transformations occur. At 448 C we start timing again at zero time; while holding at 448 C for 10 s, approximately 50 percent of the remaining unreacted 50% (or 25% of the original specimen) will transform to bainite. And upon cooling to room temperature, the remaining 25% of the original specimen transforms to martensite. Hence, the final microstructure consists of about 50% pearlite (medium), 25% bainite, and 25% martensite. (d) Cool rapidly to 398 C (671 K), hold for 2 s, then quench to room temperature.
17 Below is Figure upon which is superimposed the above heat treatment. After cooling to and holding at 400 C for 2 s, no of the transformation begin lines have been crossed, and therefore, the specimen is 100% austenite. Upon cooling rapidly to room temperature, all of the specimen transforms to martensite, such that the final microstructure is 100% martensite. (e) Cool rapidly to 398 C (671 K), hold for 20 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
18 After cooling and holding at 400 C for 20 s, approximately 40% of the specimen has transformed to bainite. Upon cooling to room temperature, the remaining 60% transforms to martensite. Hence, the final microstructure consists of about 40% bainite and 60% martensite. (f) Cool rapidly to 398 C (671 K), hold for 200 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
19 After cooling and holding at 400 C for 200 s, the entire specimen has transformed to bainite. Therefore, during the cooling to room temperature no additional transformations will occur. Hence, the final microstructure consists of 100% bainite. (g) Rapidly cool to 575 C (848 K), hold for 20 s, rapidly cool to 350 C (623 K), hold for 100 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
20 After cooling and holding at 575 C for 20 s, the entire specimen has transformed to fine pearlite. Therefore, during the second heat treatment at 350 C no additional transformations will occur. Hence, the final microstructure consists of 100% fine pearlite. (h) Rapidly cool to 250 C (523 K), hold for 100 s, then quench to room temperature in water. Reheat to 315 C (588 K) for 1 h and slowly cool to room temperature. Below is Figure upon which is superimposed the above heat treatment.
21 After cooling and holding at 250 C for 100 s, no transformations will have occurred at this point, the entire specimen is still austenite. Upon rapidly cooling to room temperature in water, the specimen will completely transform to martensite. The second heat treatment (at 315 C for 1 h) not shown on the above plot will transform the material to tempered martensite. Hence, the final microstructure is 100% tempered martensite.
22 CHAPTER 17 CORROSION AND DEGRADATION OF MATERIALS PROBLEM SOLUTIONS Electrochemical Considerations 17.1 (a) Briefly explain the difference between oxidation and reduction electrochemical reactions. (b) Which reaction occurs at the anode and which at the cathode? (a) Oxidation is the process by which an atom gives up an electron (or electrons) to become a cation. Reduction is the process by which an atom acquires an extra electron (or electrons) and becomes an anion. (b) Oxidation occurs at the anode; reduction at the cathode.
In order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationMATERIALS 101 INTRODUCTION TO STRUCTURE AND PROPERTIES WINTER Problem Set 6 Due: Tuesday, March 6, 11:00 AM
Problem Set 6 Due: Tuesday, March 6, 11:00 AM 1. TTT Diagrams Based on the transformation diagrams for eutectoid steel shown below, what microstructure would result from the following cooling histories?
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS. C Zn A Cu C Zn A Cu C Cu A Zn. (30)(63.55 g /mol) (30)(63.55 g /mol) (70)(65.
HAPTER 4 IMPERFETIONS IN SOLIDS PROBLEM SOLUTIONS wt% u? 4.7 What is the composition, in atom percent, of an alloy that consists of 30 wt% Zn and 70 4.6 as In order to compute composition, in atom percent,
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationFor Cu, which has an FCC crystal structure, R = nm (Table 3.1) and a = 2R 2 =
7.9 Equations 7.1a and 7.1b, expressions for Burgers vectors for FCC and BCC crstal structures, are of the form a b = uvw where a is the unit cell edge length. Also, since the magnitudes of these Burgers
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationHW 8. G = a 3 G v. 6a 2. Problem a. To Find:
HW 8 Problem 10. a. To Find: (a) The expression for total free energy change for a cubic nucleus, critical cube edge length, a*, and G* (b) Compare G* for a cube with that for a sphere b. Given: Nucleus
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationCHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS
191 CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS Heat Capacity 19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of the specific heat, the mass of
More informationExperiment: Heat Treatment  Quenching & Tempering
Experiment: Heat Treatment  Quenching & Tempering Objectives 1) To investigate the conventional heat treatment procedures, such as quenching and annealing, used to alter the properties of steels. SAE
More informationMATERIALS SCIENCE AND ENGINEERING
Complete Solutions to Selected Problems to accompany MATERIALS SCIENCE AND ENGINEERING AN INTRODUCTION Sixth Edition William D. Callister, Jr. The University of Utah John Wiley & Sons, Inc. Copyright 2003
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationDr. Pulak M. Pandey. paniit.iitd.ac.in/ ~ pmpandey
Dr. Pulak M. Pandey http:// paniit.iitd.ac.in/ ~ pmpandey Metals and alloys may not posses all the desired properties in the finished product. Alloying and heat treatment are two methods which are extensively
More informationMaterials Issues in Fatigue and Fracture
Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view
More informationv kt = N A ρ Au exp (
42 4.2 Determination of the number of vacancies per cubic meter in gold at 900 C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows: N v N exp Q v N A ρ Au kt A Au exp Q v kt (6.023
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationHEAT TREATMENT OF STEEL
HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice
More informationDevelopment of HighStrength Steel Wire with Superior Weldability
INDUSTRIAL MATERIALS Development of HighStrength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai Highcarbon
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationSurface Treatments. Corrosion Protective coatings for harsh environments (catalytic converters, electrochemical cells )
Surface Treatments Applications Biomedical (biocompatible coatings on implants, drug coatings for sustained release ) Mechanical Tribological friction and wear (tool steels, implants ) Fatigue minimize
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More information5 Some standard heat treatments
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
More informationCHAPTER 9 Part 1. = 5 wt% Sn95 wt% Pb C β. = 98 wt% Sn2 wt% Pb. = 77 wt% Ag23 wt% Cu. = 51 wt% Zn49 wt% Cu C γ. = 58 wt% Zn42 wt% Cu
CHAPTER 9 Part 1 9.5 This problem asks that we cite the phase or phases present for several alloys at specified temperatures. (a) For an alloy composed of 15 wt% Sn85 wt% Pb and at 100 C, from Figure
More informationSection 3: HEAT TREATMENT
Section 3: HEAT TREATMENT Introduction Objectives of Heat Treatment Heat Treatment is the controlled heating and cooling of metals to alter their physical and mechanical properties without changing the
More informationCONCEPT CHECK QUESTIONS AND ANSWERS. Chapter 2 Atomic Structure and Interatomic Bonding
CONCEPT CHECK QUESTIONS AND ANSWERS Chapter 2 Atomic Structure and Interatomic Bonding Concept Check 2.1 Question: Why are the atomic weights of the elements generally not integers? Cite two reasons. Answer:
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationRetained Austenite: NonDestructive Analysis by XRD and ASTM E Dr. Alessandro Torboli  XRay Marketing Manager
Retained Austenite: NonDestructive Analysis by XRD and ASTM E97503 Dr. Alessandro Torboli  XRay Marketing Manager Outline Introduction to XRay Diffraction Retained Austenite Retained Austenite by
More informationEffect of Heat Treatment Processes on the Mechanical Properties of Medium Carbon Steel
Journal of Minerals & Materials Characterization & Engineering, Vol. 11, No.2 pp.143152, 2012 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment Processes on the Mechanical Properties
More informationMAE 20 Winter 2011 Assignment 2 solutions
MAE 0 Winter 0 Assignment solutions. List the point coordinates of the titanium, barium, and oxygen ions for a unit cell of the perovskite crystal structure (Figure.6). In Figure.6, the barium ions are
More informationChapter 12 Elasticity
If I have seen further than other men, it is because I stood on the shoulders of giants. Isaac Newton 12.1 The Atomic Nature of Elasticity Elasticity is that property of a body by which it experiences
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationHeat Treatment of Steel
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationMet2023: Concepts of Materials Science I Sample Questions & Answers,(2009) ( Met, PR, FC, MP, CNC, McE )
1 Met223: Concepts of Materials Science I Sample Questions & Answers,(29) ( Met, PR, FC, MP, CNC, McE ) Q1.Define the following. (i) Point Defects (ii) Burgers Vector (iii) Slip and Slip system (iv)
More informationContinuous Cooling Transformation (CCT) Diagrams
Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi221
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationA8 Thermal properties of materials
A8 Thermal properties of materials Thermal properties the melting temperature, T m, and the glass temperature (temperatura de transição vítrea), T g, relate directly to the strength of the bonds in the
More informationHigh carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance
Data Sheet: A2.2 High carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance General description Steel is generally classified as high carbon steel if the nominal
More informationAlloys & Their Phase Diagrams
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationBINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)
BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A
More informationTemperature and Heat
Temperature and Heat Foundation Physics Lecture 2.4 26 Jan 10 Temperature, Internal Energy and Heat What is temperature? What is heat? What is internal energy? Temperature Does a glass of water sitting
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationINFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES
COMATTECH 2005 TRNAVA, 2021 October 2005 INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES Jiří MALINA 1+2, Hana STANKOVÁ 1+2, Jaroslav DRNEK 3, Zbyšek NOVÝ 3, Bohuslav MAŠEK
More informationObjectives/Introduction Extraction of zinc Physical properties of zinc Zinc casting alloys Wrought zinc alloys Engineering design with zinc alloys
Lecture 7 Zinc and its alloys Subjects of interest Objectives/Introduction Extraction of zinc Physical properties of zinc Zinc casting alloys Wrought zinc alloys Engineering design with zinc alloys Objectives
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 5 Heat Treatment of Plain Carbon and Low
More informationDamasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems:
Damasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems: Sharp edges on chef knives. Nitrobe 77 is dishwasher safe without risk of corrosion or edge
More informationDer Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen
Der Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen Tagung des Arbeitskreises Thermophysik, 4. 5.3.2010 Karlsruhe, Deutschland E. Kaschnitz Österreichisches GießereiInstitut
More informationFull Density Properties of Low Alloy Steels
Full Density Properties of Low Alloy Steels Michael L. Marucci & Arthur J. Rawlings Hoeganaes Corporation, Cinnaminson, NJ Presented at PM 2 TEC2005 International Conference on Powder Metallurgy and Particulate
More informationHW 10. = 3.3 GPa (483,000 psi)
HW 10 Problem 15.1 Elastic modulus and tensile strength of poly(methyl methacrylate) at room temperature [20 C (68 F)]. Compare these with the corresponding values in Table 15.1. Figure 15.3 is accurate;
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationChapter Outline. Defects Introduction (I)
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight
More informationCHROMIUM STEEL POWDERS FOR COMPONENTS. JEANETTE LEWENHAGEN Höganäs AB, Sweden
CHROMIUM STEEL POWDERS FOR COMPONENTS JEANETTE LEWENHAGEN Höganäs AB, Sweden KEYWORDS Prealloyed steel powder, chromium, PM ABSTRACT Chromium as an alloying element is of great interest due to its low
More informationPOSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H1111 Budapest, Goldmann tér 3. Summary In this
More information